Ammonium tantalum oxide fluorides: new features of dynamic disorder
Udovenko, Anatoly A.; Laptash, Natalia M.; Acta Crystallographica Section B 75 (2019) –; doi:10.1107/S2052520619013994

data_2108542
_publ_section_title
;
 Ammonium tantalum oxide fluorides: new features of dynamic disorder
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first
;
;
_journal_paper_doi               10.1107/S2052520619013994
_journal_volume                  75
_journal_year                    2019
_chemical_formula_moiety         '(N H4)3, Ta O F6'
_chemical_formula_sum            'F6 H12 N3 O Ta'
_chemical_formula_weight         365.08
_chemical_name_common            'ammonium  tantalum oxide fluoride'
_space_group_crystal_system      cubic
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.33100(10)
_cell_length_b                   9.33100(10)
_cell_length_c                   9.33100(10)
_cell_measurement_reflns_used    4131
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      38.66
_cell_measurement_theta_min      3.79
_cell_volume                     812.427(15)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_detector_area_resol_mean 8.33
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0178
_diffrn_reflns_av_unetI/netI     0.0082
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            4884
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         42.943
_diffrn_reflns_theta_min         3.782
_exptl_absorpt_coefficient_mu    13.593
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Bruker SADABS'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    2.985
_exptl_crystal_description       octahedron
_exptl_crystal_F_000             672
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.175
_exptl_crystal_size_min          0.150
_exptl_transmission_factor_max   0.748
_exptl_transmission_factor_min   0.570
_refine_diff_density_max         0.230
_refine_diff_density_min         -0.254
_refine_diff_density_rms         0.041
_refine_ls_extinction_coef       0.0082(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.167
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     22
_refine_ls_number_reflns         191
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.167
_refine_ls_R_factor_all          0.0059
_refine_ls_R_factor_gt           0.0059
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0081P)^2^+0.0421P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0139
_refine_ls_wR_factor_ref         0.0139
_reflns_Friedel_coverage         0.000
_reflns_number_gt                191
_reflns_number_total             191
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            wf5152sup1.cif
_cod_data_source_block           I
_cod_original_cell_volume        812.43(3)
_cod_database_code               2108542
_shelx_estimated_absorpt_t_min   0.172
_shelx_estimated_absorpt_t_max   0.235
_shelx_res_checksum              66504
_shelx_hkl_checksum              10338
_cod_database_fobs_code 2108542